## DEFORMATION AND FAILURE ANALYSIS OF SYMMETRIC AND

## ANTI-SYMMETRIC GRAPHITE/EPOXY LAMINATE DUE TO VARIATIONS IN

## FIBER ORIENTATION

Azizul Hakim Samsudin, Ahmad Kamil Hussain and Jamaluddin Mahmud

Faculty of Mechanical Engineering, Universiti Teknologi MARA, Shah Alam, Selangor, Malaysia E-Mail: [email protected]

**ABSTRACT **

This paper aims to simulate and analyse the failure behaviour, deformation behaviour and mode of failure of composite laminate using the built-in failure criteria function provided by ANSYS. Finite element modelling and analysis of symmetric and anti-symmetric Graphite/ Epoxy laminate with various angles of fiber orientation subjected to uniaxial tension are performed. Maximum Stress Theory and Tsai-Wu Failure Criteria are employed to determine the failure load (failure index = 1). Prior to that, numerical validation and convergence analysis are carried out. The failure loads (First ply failure, FPF and last ply failure, LPF loads) and corresponding stresses (σx, σy and τxy) predicted from the finite element simulation using ANSYS are then transformed to determine the principal stresses (σ1, σ2 and τ12) using a MATLAB programme, specifically developed for stress transformation computation. Principal stresses are then used to determine the modes of failure (fiber failure, matrix failure or shear stress) of each layer corresponding to specific angle of fiber orientation. The failure curves (FPF and LPF) for both laminates (symmetric and anti-symmetric) and both theories (Maximum Stress Theory and Tsai-Wu) are plotted and found to be very close to each other. Therefore, it can be concluded that the current study is useful and significantin enhancing knowledge about the failure behaviour, deformation behaviour and mode of failure of composite laminate.

**Keywords:** ccomposite laminate, deformation analysis, failure analysis, ANSYS.

**INTRODUCTION**

Composite materials are increasingly used in the construction of mechanical, aerospace, marine and automotive structures since they offer improved material properties and high strength-to-weight ratio. The other main advantage is that its stiffness and strength can be tailored to specific design loads. The capability of composite structure to withstand critical loading can be evaluated either by physical testing or any advance computational method.

Experimental approach (physical tests) required to establish strength characteristics of composite materials are complex, tedious and expensive. This is because to come up with an accurate assessment of a lamina design requires many repetitive tests and sufficient number of samples to cater changes in material properties, lamination scheme, and loading conditions.

Therefore the idea of failure theory has been
introduced to predict the strength of a composite materials
(Khashaba *et al.*, 2013), (Liu and Zheng, 2010), (Taha and
Shrive, 2006). Theoretically, determining the desired
strength of composite laminate has involved complex
computational method and highly mathematical
implementation. Thus to avoid this, the current usual
preferred analytical tool is the finite element (FE)
implementation using commercial software (Zhang and
Yang, 2009).

Predicting tool is important, driven by the observation that extensive tests on composite structures are extremely expensive (Nahas, 1986). This is because to

requires many repetitive calculations due to changes in
loading conditions, material properties, and laminate
geometry (Rahimi *et al*., 2012).

In developing the FE model of composite
laminates, scientists or engineers use programming
languages, computational tools and algorithms to create
codes that run efficiently on high performance computers
(Tay *et al*., 2008). Moreover, at present there are digital
computers and software packages that could perform
laminate analysis that can satisfy various computational
requirements for solution.

Failure occurs in a material when the applied load reached its threshold. For composite laminate failure in any one layer does not imply failure of other layers in other directions. Therefore it is important to study the behaviour of composite laminate after failure (progressive failure) that occurred in a lamina with the ply by ply approach which considered as bonded layers (Nahas, 1986).

Laminated composite structures develop local
failures such as matrix cracks, fibre breakage fibre matrix
and ply delamination under normal operating conditions,
which are termed as damage (Gupta, *et al*., 2013), (Wang
*et al*., 2013). All of those could occur in any ply in the
laminate and the weakest which fails first is considered as
the first ply failure (FPF). These effect cause permanent
loss of integrity within the laminate and result in loss of
stiffness and strength of the material. The failure will
further propagate to the next weakest plies available until
it finally leads to the total rupture when the last ply fails
(Nahas, 1986). While the first ply failure analysis often
overlooks the consequence of individual failure,
determination of last ply failure (LPF) depends greatly on
it.

In terms of failure criterion, Maximum Stress
Theory is one of the famous failure criteria employed in
predicting composite laminate failure (Sun *et al*., 1996),
(Pedro, 2002). Maximum Stress Theory considers that the
composite fails when the stress in the principal material
axes (σ1, σ2 and τ12) exceeds the corresponding strength in
that direction (exceeds the respective allowable). It is
simple and direct way to predict failure of composites and
no interaction between the stresses acting on the lamina is
considered. Failure will occur when any one of the stress
components fails.

Another commonly employed is the Tsai-Wu
failure criterion, where it involves polynomial composite
laminate in predicting composite failure. However,
Tsai-Wu cannot identify modes of failure (fiber failure, matrix
failure and shear stress) compared to interactive failure
criteria, such as the Maximum Stress Theory (Nahas,
1986), (Rahimi *et al.*, 2012). In general, due to its form,
the Tsai-Wu failure criterion could identify an element
failure (Padhi *et al.*, 1998).

Previous study focused on predicting the first ply
failure and last ply failure of composite laminates (Rahimi
*et al.*, 2012). Nevertheless, the deformation behaviour and
mode of failure have not been analysed thoroughly,
although the deformation behaviour and mode of failure of
composite laminates are indeed very interesting
phenomena. For example, for a two-layer laminate, the
deformation behaviour could be different for both
symmetric and anti-symmetric laminate under variations of
fiber angle orientation and this phenomenon has not been
thoroughly investigated.

Therefore, this study aims to predict the failure behaviour, deformation behaviour and mode of failure of two-layer symmetric and anti-symmetric graphite/epoxy

laminate under uniaxial tension due to variations of fiber angle orientation.

**METHODOLOGY **

In order to achieve the main objectives of this study, the current study is carried out in four main stages:

**Stage 1:** Numerical validation and convergence analysis
**Stage 2:** Failure analysis

**Stage 3:** Deformation analysis
**Stage 4:** Mode of failure analysis.

Figure-1 shows the overall workflow of the
current study. The workflow repeated with different
variations in angle (0o_{, 10}o_{, 20}o_{, 30}o_{, 40}o_{, 45}o_{, 50}o_{, 60}o_{, 70}o_{, }
80o_{, 90}o_{) and using two failure criteria (Maximum Stress }
Theory and Tsai-Wu).

**Figure-2.** Geometry and computational domain for
composite laminate under transverse load.

**Numerical Validation **

The current finite-element results (ANSYS) have been validated by comparing to the exact solution. The

plate geometry is shown in Figure-2 and the material properties are tabulated in Table-1. The results are good since the error is found less than 2% (Table-2).

**Table-1.** Material properties of T300/5208 graphite/epoxy.

**Properties Values **

E1 132.4 GPa

E2= E3 10.76 GPa G12 = G13 5.65 GPa

G23 3.38 GPa

12 = 13 0.24

23 0.49

Ply thickness, *h*i 0.127mm/ply

**Table-2.** Comparison of exact and finite-element solution, z-displacement (mm)
for laminated composite plate (229mm by 127mm).

**Lamination scheme ** **UDL **
(Pa)

**Exact **
**Solution **

(mm)

**ANSYS **
(mm)

**Error **
(%)

[ 0/ 90/ 0/ 90]T 689.5 0.00340 0.00338 0.59 [ 0/ 90/ 90/ 0]T 689.5 0.00582 0.00579 0.52 [45/-45/45/-45]T 689.5 0.00276 0.00274 0.72 [15/-15/15/-15]T 689.5 0.00639 0.00636 0.43 [ 45 / -45 ]T 689.5 0.04066 0.04029 0.91 [ 15 / -15 ]T 689.5 0.06610 0.06576 1.42

**Convergence Analysis **

A major bottleneck in the finite element process
is that of mesh size. Smaller the mesh size, the higher the
accuracy of the predicted results but it will increased the
computing time (Liu *et al*., 2011). This justify that
convergence analysis is important. Thus, this study starts
with convergence analysis. These analyses are done using
mapped meshing (2x2, 4x4, 8x8. 16x16, 32x32, 64x64,
128x128 and 256x256) with quadrilaterals element under
constant uniaxial tension (7010.5 N). Mesh size of 1x1 (or
any odd mesh size) is not possible as the boundary
condition is fully fixed at the centre of the plate.

Figure-3 shows that constant stresses are generated for both symmetric laminate and anti-symmetric laminate.

**Figure-3.** Computed stress (symmetric and
anti-symmetric) at various fiber orientation.

analyses are carried out (failure analysis, deformation analysis and mode of failure analysis).

**Figure-4.** Displacement in x-direction for symmetric
[/]T laminate.

**Figure-5.** Displacement in x-direction for anti-symmetric
[/-]T laminate.

**Failure and Deformation Analysis of Composite **
**Laminate **

Symmetric and anti-symmetric composite plates
are modelled as shown in Figure-6 under uniaxial tension.
The laminate is made of two layer, and for this study two
lamination schemes are analysed, where the layup are
symmetry (/)T and anti-symmetry (/-)T. The plate is
rectangle, with a thickness of 1.27x10-4_{m/ply and made of }
graphite-epoxy. The material and strength properties are
shown in Table-3.

A finite element failure analysis procedure is carried out using commercial software (ANSYS v15.0, 2013 SAS IP, Inc.). The predictions of failure are based on available built in failure theory and failure criteria functions which are Maximum Stress Theory (equation 1) and Tsai-Wu (equation 2). The deformation behaviour is also recorded during the failure.

**Figure-6.** Uniaxial tension model.

**Table-3.** Material properties for T300/5208 (J.N.
Reddy *et al.,* 1987).

**E****1****= 138 GPa ** **X****T****= 1035 MPa **

*E2* = 10.6 GPa *XC* = 1035 MPa

12 = 0.3 *YT* = 27.6 MPa
*G12* = 6.46 GPa *YC* = 138 MPa

*S * = 41.4 MPa

σ1 = Xt or Xc, σ2 = Yt or Yc, τ12 = S (1)

F1σ1 + F2σ2 + F6τ12 + F11σ12+F22σ22+2F12σ1σ2 + F66τ212 ≥ 1(2)

**Mode of Failure Analysis**

Since the stresses predicted using ANSYS are computed for global axis (σx, σy and τxy), a programme based on transformation matrix equation is developed using MATLAB (v8.1.0.604, R2013a, The MathWorks, Inc.) to determine the principal stresses (σ1, σ2 and τ12) for every angle. The used of stress transformation equation (equation 3) in order to determine the principal stresses. Principle stresses are then used to categorize each of the angles in failure mode based on theoretical calculation (fiber failure, matrix failure or shear failure).

*xy*
*y*
*x*
2
2
2
2
2
2
12
2
1
sin
cos
cos
sin
cos
sin
cos
sin
2
cos
sin
cos
sin
2
sin
cos
(3)
**RESULTS **

**Figure-7.** Failure curves for symmetric [/]T laminate
(Maximum Stress Theory and Tsai-Wu).

Results for symmetric laminate (Figure-8) show
the deformation behaviour (x-directions) during failure as
predicted by Maximum Stress Theory and Tsai-wu.
Displacement in x-direction shows that Maximum Stress
Theory predicts higher displacement than Tsai-wu but at
angle 0o_{ and 90}o_{ the displacement are the same. At angle }
0o_{, the plate deformed the longest since the fibre direction }
parallel to the x-axis (global axis) which also the direction
of load being applied. While the less deformed plate occur
at angle 90o_{ since the fibre direction perpendicular to the }
x-axis (global axis) which also perpendicular to the load
applied. This makes the plate easier to break.

**Figure-8.** Displacement (x-direction) curves for symmetric
[/]T laminate (Maximum Stress

Theory and Tsai-Wu).

It goes the same with displacement in y-direction
where Maximum Stress Theory predicts more
displacement than Tsai-Wu and also at angle 0o_{ and 90}o
the displacement are the same. For both Maximum Stress
Theory and Tsai-Wu predicts the highest displacement
occur at angle 10o_{ while the lowest displacement predicted }
at angle 90o_{. }

**Figure-9.** Displacement (y-direction) curves for symmetric
[/]T laminate (Maximum Stress

Theory and Tsai-Wu).

From the observation in Figure-8 and Figure-9, it can be concluded that Tsai-Wu predicts a smoother curve than Maximum Stress Theory, thus proving that the interaction terms between the stresses (σx and σy) are significant. For symmetric laminate, the failure predicted at the same stress since the fiber orientation for both layers are the same.

**Table-4.** Mode of failure for symmetric [/]T laminate.

**Modes of **
**failure / **
**Angle (o _{) }**

**Isometric View **

Fiber Failure
(XT)
(0o_{ to 2}o_{) }

Shear Failure

(S)
(3o_{ to 33}o_{) }

Matrix
Failure
(YT)
( 34o_{ to 90}o_{ ) }

For anti-symmetric laminate (Figure-10), it could
be observed that there is no significant difference of the
failure curves between Tsai-Wu and Maximum Stress
Theory, except between angle 10o_{ until 70}o_{ fiber }
orientation. The failure curves for the 70o_{ to 90}o
orientation are almost similar. Comparing between the
failure curves of Maximum Stress Theory and Tsai-Wu, it
is found that failure curves of shear stress (mode of failure
- Table-5) shows different value of stresses while at the
fibre failure and matrix failure does not shows any
different. For anti-symmetric laminate, the failure
predicted at the same stress since there is no different
between angle positive and negative fibre orientation.

**Figure-10.** Failure curves for anti-symmetric [/-]T
laminate (Maximum Stress Theory and Tsai-Wu).

Figure-11 shows the deformation behaviour
(x-directions) during failure as predicted by Maximum Stress
Theory and Tsai-wu. Displacement in x-direction shows
that Maximum Stress Theory predicts higher displacement
than Tsai-wu but at angle 0o_{ and 90}o_{ the displacement are }
the same.

**Figure-11.** Displacement (x-direction) curves for
anti-symmetric [/]T laminate (Maximum Stress Theory

and Tsai-Wu).

**Figure-12.** Displacement (y-direction) curves for
anti-symmetric [/-]T laminate (Maximum Stress Theory

and Tsai-Wu).

Figure-13 shows the deformation behaviour
(z-directions) during failure as predicted by Maximum Stress
Theory and Tsai-wu. Displacement in x-direction shows
that Maximum Stress Theory predicts higher displacement
than Tsai-wu but at angle 0o_{ and 90}o_{ the displacement are }
the same.

**Figure-13.** Displacement (z-direction) curves for
anti-symmetric [/-]T laminate (Maximum Stress Theory

and Tsai-Wu).

Table-5 shows the range of angle between the
modes of failure (referring to principal stresses σ1, σ2 and
τ12) obtained using MATLAB programme based on stress
transformation equation. It shows that fiber failure occur
between angle 0o_{ to 2}o_{ while the remaining is shear stress }
(3o_{ to 48}o_{) and matrix failure (49}o_{ to 90}o_{). The simulation }
results clearly show that anti-symmetric laminate
experience twisting deformation under uniaxial tension.

**Table-5.** Mode of failure for anti-symmetric [/-]T
laminate.

**Modes of **
**Failure / **
**Angle (o _{) }**

**Isometric View **

Fibre Failure
(XT)
( 0o_{ to 2}o_{ ) }

Shear Failure
(S)
( 3o_{ to 48}o _{) }

Matrix
Failure
(YT)
( 49o_{ to 90}o_{ ) }

**CONCLUSIONS **

This paper presented the application of numerical analysis using commercial software (ANSYS) and MATLAB programme to predict the failure of composite laminates under uniaxial tension, to predict the deformation behaviour of the composite laminate during failure and finally to determine the mode of failure due to variations in angle of fiber orientation.

The results of the study prove that the main objective of the research to predict the failure curves and deformation behaviour of composite laminate using a novel approach has been achieved successfully. Modes of failure on each angle variations are also predicted.

Thus, it can be concluded that the current study is useful and contributes significant knowledge to the failure behaviour of composite laminate.

**ACKNOWLEDGEMENT **

This work is supported by Universiti Teknologi MARA (UiTM) and Ministry of Education (MOE) Malaysia under the Fundamental Research Grant Scheme (grant no 600 - RMI/FRGS 5/3 (80/2014)).

**REFERENCES **

[1] Nahas, M.N. 1986. Survey of failure and post-failure theories of laminated fiber-reinforced composites, Journal of Composites Technology and Research. 8, pp. 138-153.

[2] Rahimi, N., Musa, M., Hussain A.K. and Mahmud J. 2012. Finite element implementations to predict the failure of composite laminate under uniaxial tension. Advanced Materials Research. 499, pp. 20-24.

[3] Mahmud, J., Ismail, A.F. and Pervez, T. 2005. Employing a failure criterion with interaction terms to simulate the progressive failure of carbon-epoxy laminate. IEM Journal, the Institution of Engineers (IEM) Malaysia, 66(2), pp. 6-14.

[4] Rahimi, N., Hussain, A.K., Meon, M.S. and Mahmud, J. 2012. Capability assesment of finite element software in predicting the last ply failure of composites laminate. Procedia Engineering. 41, pp.1647-1653.

[5] Liu, W., Geni, M. and Yu, L. 2011. Effect of mesh size of finite element analysis in modal analysis for periodic symmetric struts support. Key Eng. Material. 462, pp. 1008-1012.

[6] Rahimi, N., Rahim, M.A., Hussain, A.K. and Mahmud, J. 2012. Evaluation of failure criteria for composite plates under tension. IEEE Symposium on Humanities, Science and Engineering Research (SHUSER 2012). pp. 849-854.

[7] Reddy, J.N. and Pandey, A.K. 1987. A first ply failure analysis of composite laminate. Computer and Structures. 25(3), pp. 371-393.

[8] Din, M.I.M., Adnan, Z.A.M. and Mahmud, J. 2014. Failure Analysis of Composite Laminates under Biaxial Tension: A Review and Framework. Applied Mechanics and Materials. 680, pp.160-163.

[9] Liu, P. F. and Zheng J. Y. 2010.Recent developments on damage modeling and finite element analysis for composite laminates: A review. Material and Design. 31, pp. 3825-3834.

[10] Khashaba, U.A., Sebaey, T.A. and Alnefaie, K.A. 2013. Failure and reliability analysis of pinned-joints composite laminates: Effects of stacking sequences. Composites Part B: Engineering. 45(1), pp. 1694-1703.

[11] Taha, M.M.R. and Shrive, N.G. 2006. A Model of Damage and Creep Interaction in a Quasi-Brittle Composite Material under Axial Loading. Journal of Mechanics. 22(4), pp. 339-347.

[12] Tay, T.E., Liu, G., Tan, V.B.C., Sun, X.S. and Pham, D.C. 2008. Progressive Failure Analysis of Composites. Journal of Composite Materials. 42, pp. 1921-1929.

[13] Zhang, Y.X. and Yang, C.H. 2009. Recent developments in finite element analysis for laminated composite plates. Composite Structures. 88, pp. 147-157.

[14] Vallejo, M.J. and Tarefder, R.A. 2011. Predicting Failure Behavior of Polymeric Composites Using a Unified Constitutive Mode. Journal of Mechanics, 27(3), pp. 379-388.

[15] Gupta, A.K., Patel, B.P. and Nath, Y. (2013). Continuum damage modeling of composite laminated plates using higher order theory. Composite Structures, 99, pp. 141-151.

[16] Wang, P., Lei, Y. and Yue, Z. 2013. Experimental and numerical evaluation of the flexural properties of stitched foam core sandwich structure. Composite Structures. 100, pp. 243-248.

[17] Sen, F. and Sayman, O. 2011.Failure Response of Two Serial Bolted Joints in Composite Laminates. Journal of Mechanics. 27(3), pp. 293-30.

[19] Hou, X., Hu, H. and Silberschmidt, V. 2014.Numerical analysis of composite structure with in-plane isotropic negative Poisson’s ratio: Effects of materials properties and geometry features of inclusions. Composites Part B: Engineering. 58, pp. 152-159.

[20] Cárdenas, D., Elizalde, H., Marzocca, P., Abdi, F., Minnetyan, L. and Probst, O. 2013.Progressive failure analysis of thin-walled composite structures. Composite Structures. 95(1), pp. 53-6.

[21] Padhi, G.S., Shenoi, R.A., Moy, S.S.J. and Hawkins, G.L. 1998. Progressive failure and ultimate collapse of laminated composite plates in bending. 40, pp. 277-291.

[22] Sun, C.T., Quinn, B.J., Tao, J. and Oplinger, D.W. 1996. Comparative Evaluation of Failure Analysis Methods for Composite Laminates, Office of Aviation Research Washington, D.C. pp. 1-133.